Presentation on theme: "Department of Chemistry University of Oslo Centre for Materials Science and Nanotechnology (SMN) FERMIO."— Presentation transcript:
email@example.com http://folk.uio.no/trulsn Department of Chemistry University of Oslo Centre for Materials Science and Nanotechnology (SMN) FERMIO Oslo Research Park (Forskningsparken) KJM5120 and KJM9120 Defects and Reactions Truls Norby Ch 4. Impurities and dopants
Impurities and dopants Foreign atoms can dissolve interstitially or substitutionally. At small concentrations they are usually called dopants or impurities, depending on whether they are added on purpose or not. For dopants that are added to substitute native atoms – especially to larger levels - we also use the term substituent. We may refer to all of these as a solute (and the host structure as the solvent.
Impurities and dopants Substituents that have the same valence as the native atom they replace are called homovalent. Substituents that have a different valence than the native atom they replace are called aliovalent or heterovalent. Foreign atoms can affect the materials property by introducing mechanical strain if the size does not fit exactly, and by introducing charged defects. Here we will consider mainly foreign atoms that fulfil their valence by accepting electrons (acceptors) or donating electrons (donors). This comprises interstitially dissolved foreign atoms and aliovalent substitutionally dissolved foreign atoms.
Foreign atoms may or may not be present in equilibrium concentrations The defect chemistry is mainly a repetition from earlier chapters – extended into more focus on foreign atoms that form charged defects. Before starting on the defect chemistry, we shall consider the dissolution reaction as being at equilibrium or not. We shall put this into some kind of system… As example, we consider the dissolution of the foreign cation Mf from a source of MfO a into the host oxide MO b.
1. Not equilibrium: The solute is frozen in. because the temperature is too low: The solute Mf can effectively not diffuse between the source/sink phase MfO a and the host structure MO. a) If the frozen concentration of solute is below the solubility limit, and no second phase is present, the system is then stable. If equilibrium was allowed (e.g. by waiting very long, or increasing the temperature a little) nothing would happen – the source is empty. b If the concentration of solute is below the solubility limit, but a second solute-rich phase is present, the system is metastable. If equilibrium was allowed, more solute would dissolve. c) If the frozen concentration of solute exceeds the solubility limit, the system is metastable – a common case. If equilibrium was allowed, solute would precipitate.
2. Equilibrium: The solute is mobile. because the temperature is high enough: The solute Mf can effectively diffuse between the source/sink phase MfO a and the host structure MO b. a)The total amount of solute present is below the solubility limit. -In this case the source is empty, and the concentration of solute is therefore again constant, as in all the cases 1). b)The total amount of solute present is above the solubility limit. -In this case there is source/sink MfO a present, and the concentration of solute is variable by exchange of solute between the bulk and the source/sink of second phase. Only for this last case (2b) does it usually make sense to treat the doping defect reaction as an equilibrium. For all the other cases that reaction will be just a way of describing how you add or substitute (and charge compensate) a certain amount of solute which thereafter is considered constant. Be aware of this…it will save you much trouble preventing you from trying to incorporate that equilibrium when you don’t need it!
We start by considering constant solute concentrations …because they are frozen (all cases 1), or because they are fully soluble way below the solubility limit (case 2a). We will often not even bother to write a defect reaction for the dissolution of the foreign species – we just state that the defects of the dissolved solute are there, in addition to the native defects.
Schottky dominated metal halide MX doped with higher valent metal halide MfX 2 Electroneutrality comprising native defects and foreign species: Schottky equilibrium: Simplified limiting cases: Intrinsic: Extrinsic (doped): Minority defect: This is a kind of Brouwer diagram, but vs the concentration of dopant
Oxygen deficient oxide substituted with lower-valent cation Most important example! Total electroneutrality: Limiting cases: The good old.. and at higher pO 2 … Check that you understand (from Ch. 3) how to obtain the pO 2 -dependencies!
Metal-deficient oxide doped with lower valent cations Example: Singly charged metal vacancies in M 1-x O! Doped with an acceptor. Concentrate on seeing qualitatively the native defects (here at high pO 2 ) and how the dopant takes over (here at lower pO 2 ) enhancing the oppositely charged defect (here holes) and suppressing the defect (here the ionic point defects) with the same charge as itself.
Metal-deficient oxide doped with lower valent cations Same oxide with singly charged metal vacancies in M 1-x O. Now doped with a donor. Note how the doping here enhances the ionic point defect and may make the material an ionic conductor, while the electronic defects go through a n=p minimum.
Doping of oxides which may have regions with both oxygen and metal deficit Example: M 2-x O 3-y Dope with lower valent Ml 2+
Doping of oxides which may have regions with both oxygen and metal deficit Example: M 2-x O 3-y Dope with higher valent Mh 4+
Full Brouwer diagrams of doped compounds We have seen two examples of Brouwer diagrams for doped oxides over entire range of pO 2. They show a few common features that the experienced defect chemist (you?) recognises and uses: Oxygen over- and under-stoichiometry dominate at high and low pO 2, as in the undoped oxides. The “intrinsic disorder” region in the middle is expanded and dominated by the dopant. This part is split in one compensated by an electronic defect and one compensated by an ionic defect. With acceptor doping the oxide becomes a p- type electronic conductor at high pO 2, and ionic at low pO 2. With donor-doping the material becomes an n- type electronic conductor at low pO 2 and an ionic conductor at high pO 2.
Full Brouwer diagrams of doped compounds When is the doped oxide stoichiometric? When the concentrations of the cation and anion vacancies are equal so that the composition is the same as in the stoichiometric host structure? –(identify this point in each diagram) Or when the concentrations of electrons and holes are equal (n = p) so that the average valence of the host structure corresponds to that in the stoichiometric host structure? –(identify also this point in each diagram) Answer: It is a matter of choice.
Variable concentration of solute High temperatures, solute present in second phase (source/sink). Case 2b Now, the dissolution reaction itself contributes an equilibrium that must be satisfied and not just a constant value of the dissolved solute.
Doping M 2 O 3 with excess MlO Consider the situation at high pO 2 where Ml 2+ substitutes M 3+ and is compensated by electron holes: Equilibrium coefficient: Electroneutrality and insertion gives: Solubility of MlO increases with pO 2 1/8 ! a MlO(s) = 1
Doping M 2 O 3 with excess MlO At lower pO 2, Ml 2+ is compensated by oxygen vacancies: Equilibrium coefficient: Electroneutrality and insertion gives: Solubility of MlO is now independent on pO 2 ! a MlO(s) = 1
Doping M 2 O 3 with excess MhO 2 At low pO 2 Mh 4+ substitutes M 3+ and is compensated by electrons: Equilibrium coefficient: Electroneutrality and insertion gives: Solubility of MhO 2 increases with decreasing pO 2 ! At higher pO 2 : Compensation by ionic defect; independent of pO 2. a MhO2(s) = 1
Hydrogen as a dopant Hydrogen can dissolve as protons H +, atoms H, molecules H 2, or hydride ions, H -. We here consider only protons, H +. We have earlier learnt that protons in oxides dissolve interstitially as H i. or, equivalently, OH O. defects. H 2 O can act as a dopant oxide for protons, H +, The concentration can be frozen, as for other foreign atoms. If at equilibrium in contact with water vapour, this water vapour is the source and sink. Its activity can be represented by pH 2 O and is thus variable. We can also use H 2 gas as source of protons (which would correspond to using metal as source for a dopant cation). H 2 and H 2 O are in equilibrium via H 2 (g) +1/2 O 2 (g) = H 2 O(g)
Protons in oxygen deficient oxide, e.g. M 2 O 3-d Hydrogen as source Water vapour as source Equilibrium coefficient If protons and electrons dominate:
Effect of water vapour on acceptor- doped M 2 O 3 Electroneutrality: Equilibrium: Limiting cases: Can you derive the pH 2 O- dependencies of the minority defects?
Variable solubility of acceptor compensated by protons Dissolution of acceptor and charge compensating protons: Electroneutrality inserted into the equilibrium coefficient yields: In other words; The solubility of acceptors compensated by protons increases with pH 2 O 1/4.
Defect – dopant association Electrostatic and mechanical relaxations bind defects together. Example: Immobilises charged defects
Concluding remarks This chapter brought mostly repetition and training of what you learned in Ch. 3. In addition you have familiarised yourself with many aspects of foreign atoms in host lattices. Check your understanding of the terms: –Solutes, impurities, dopants, substituents. –Interstitial vs substitutional foreign atoms –Acceptor vs donor solutes/dopants/impurities/substituents –Homovalent vs heterovalent (aliovalent) substituents –Equilibrium concentration of solutes vs Frozen concentration of solutes (reason?) –Variable vs constant concentration of solutes (reasons?) Being able to draw a Brouwer diagram for a given native defect pair and the adding a donor or acceptor level and sketching its impact on the two native defects is good, Being able to draw the entire Brouwer diagram across all defect situations is even better.
Outlook This concludes our lectures in defect chemistry. It should enable you to derive expressions for the concentration of defects as a function of temperature, pO 2, pH 2 O, and doping type and concentration. The next Chapter (5) treats random diffusion of species; atoms, ions, and defects. The diffusivity of atoms and ions requires defects and is thus proportional to the concentration of defects. Chapter 6 treats random diffusion in an electrical field, giving rise to currents and the term electrical conductivity. Conductivity is proportional to the concentration of defects. Chapter 7 finally couples two types of transport – typically ionic and electronic – into solid state electrochemistry. Here we meet terms such as chemical diffusion, ambipolar diffusion, creep, sintering, reactivity, corrosion, permeability, and applications such as fuel cells, electrolysers, sensors, and gas separation membranes.